Linker Installation: Engineering Pore Environment with Precisely Placed Functionalities in Zirconium MOFs.
Yuan, Shuai; Chen, Ying-Pin; Qin, Jun-Sheng; Lu, Weigang; Zou, Lanfang; Zhang, Qiang; Wang, Xuan; Sun, Xing; Zhou, Hong-Cai; Journal of the American Chemical Society 138 (2016) 8912–8919; doi:10.1021/jacs.6b04501

data_4125136
_publ_section_title
;
 Linker Installation: Engineering Pore Environment with Precisely Placed
 Functionalities in Zirconium MOFs.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              8912
_journal_page_last               8919
_journal_paper_doi               10.1021/jacs.6b04501
_journal_volume                  138
_journal_year                    2016
_chemical_formula_moiety         '[Zr6 O8 O8] [(C18 H16 O4)4]'
_chemical_formula_sum            'C72 H64 O32 Zr6'
_chemical_formula_weight         1988.55
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           131
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4c 2'
_symmetry_space_group_name_H-M   'P 42/m m c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   24.218(10)
_cell_length_b                   24.218
_cell_length_c                   15.359(6)
_cell_measurement_reflns_used    1657
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      17.7952
_cell_measurement_theta_min      2.3010
_cell_volume                     9008(5)
_computing_cell_refinement       'SAINT+ ver. (Bruker, 2001)'
_computing_data_collection       'APEX2  (Bruker, 2008)'
_computing_data_reduction        'SAINT+ ver. (Bruker, 2001)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  'SHELXTL (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1914
_diffrn_reflns_av_sigmaI/netI    0.1297
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -30
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            52981
_diffrn_reflns_theta_full        26.41
_diffrn_reflns_theta_max         26.41
_diffrn_reflns_theta_min         1.68
_exptl_absorpt_coefficient_mu    0.371
_exptl_absorpt_correction_T_max  0.9638
_exptl_absorpt_correction_T_min  0.9638
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2008)'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    0.733
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Blocky
_exptl_crystal_F_000             1984
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.10
_platon_squeeze_details
;
;
_refine_diff_density_max         0.744
_refine_diff_density_min         -0.518
_refine_diff_density_rms         0.061
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.004
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     130
_refine_ls_number_reflns         5011
_refine_ls_number_restraints     19
_refine_ls_restrained_S_all      1.002
_refine_ls_R_factor_all          0.1586
_refine_ls_R_factor_gt           0.0582
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0300P)^2^+3.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1079
_refine_ls_wR_factor_ref         0.1210
_reflns_number_gt                2302
_reflns_number_total             5011
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja6b04501_si_003.cif
_cod_data_source_block           PCN700Me4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 4125130--4125148.cif.
;
_cod_original_sg_symbol_H-M      P42/mmc
_cod_database_code               4125136